“Advanced Physical Metallurgy”
‐ Bulk Metallic Glasses ‐
Eun Soo Park
Telephone: 880‐7221 Email: email@example.com
Office hours: by appointment
4.6 Bulk Metallic Glass Casting Methods
4.6.1 Water‐Quenching Method: CR~ about 10‐100 K/s
4.6.2 High‐Pressure Die Casting
: offer high solidification rates high productivity, low casting defect, and possible to produce more complex shapes even in alloys with a high viscosity
4.6.6 Squeeze‐casting Method
: Push the molten alloy through hydraulic high pressure into the Cu mold until the liquid alloy completely solidified → Undercooling to much below the equilibrium solidification temperature
4.6.3 Copper Mold Casting : most common and popular method to produce BMGs: Injection casting, Centrifugal casting, Strip casting, Arc melting, Suction casting, tilt‐
casting, Cap‐cast technique (bringing a metallic cap into contact with the molten metal, and applied a small pressure of about 1 kN → high CR)
→ Automatic Production Process of BMGs(Human error ↓ & Homogeneity ↑)
4.6.8 Unidirectional Zone Melting Method 4.6.9 Electromagnetic Vibration Process
: destroy clusters of strong local order → GFA↑
4.8 Mechanical Alloying → Extrusion or Spark Plasma Sintering(multi‐step process) : used to easily produce amorphous phases in those systems where conventional
melting and casting methods prove difficult or impossible (wide composition ranges)
4.7 Bulk Metallic Glass Composites
: exhibit much better mechanical properties → detail later in Chapter 8
BMG matrix composites
Solidification from the melt
dendritic or special shape (nm/μm-size) Quasicrystalline precipitates:
(nm/μm-size) Amorphous precipitates:
Addition of insoluble particles (1) to the melt or (2) to the powder + consolidation
Partial devitrification of BMGs via annealing/
severe deformation Fibers
dendritic or special shape (nm/μm-size)
(nm/μm-size) Quasicrystalline precipitates:
Eckert at al, Adv Eng Mater 2007
IH4 Spinodal Decomposition?
Formation of a composite microstructure within a single production step
a), b) Crystalline precipitates
c) Quasicystalline precipitates
d) Two phase amorphous
4.7.1 In Situ Composites: usually produced by adjusting the chemical composition of the alloy : Shape of crystalline phase_usually dendritic → homogenized in the mushy (liquid+
soild) region_spherical shape → further improve the mechanical properties
1) Solidification : preciipitation of primary ductile phase
(Johnson et al., Acta Mater., 2001)
2) Solidification : precipitation of ductile phase
Ta rich particle (Johnson et al., Acta Mater., 2001)
Douglas C. Hofmann, SCIENCE VOL 329 10 SEPTEMBER 2010
4.7.2 Ex Situ Composites: usually very large volume fraction of second crystalline phase _ type of reinforcements_pure metals (tungsten, molybdenum, tantalum, nickel,
copper and titanium), alloys (1080 steel, stainless steel, and brass), and non‐
metallics (SiC, diamond, and graphite)
For example: Melt‐infiltration technique for the case of long and continuous fibers
1) Casting : hard/ductile particle
2) Extrusion : ductile powder
0.00 0.01 0.02 0.03 0.04 0.05 0.06 0.07 0.08 0.09 0.10 0
500 1000 1500 2000 2500 3000
Max. compressive strength: 2.05 GPa Total strain: 2.8 %
Plastic strain: 0.8 %
Max. compressive strength: 1.64 GPa Total strain: 4.7 %
Plastic strain: 2.7 %
strain rate at room temp. = 6x10-5s-1
Max. compressive strength: 2.44 GPa
(Johnson et al., Acta Mater.,1999)
(Kim et al., J. Non-cryst. Solids, 2002)
4.9 Bulk Metallic Glass Foams
:have interesting combination of properties such as high stiffness in conjunction with very low specific weight, high gas permeability combined with high thermal conductivity, high mechanical energy absorption, and good acoustic damping.
→ Pores as a gaseous second phase_equally effective in inhibiting catastrophic failures resulting from shear band localization
Pore sizes ranging from the sub‐micrometer to the millimeter scale and porosities ranging from 2% to more than 85%
Review of the state of the art in the processing of BMG foams I
· Pd43Cu27Ni10P20: produced by expansion in the liquid alloy of water vapor bubbles generated from hydrated boron oxide flux powders, followed by quenching.
Schematic drawing of the eggbeater constructed for the mechanical air‐
The setup comprises a molybdenum brush of 3 cm diameter spinning at
speeds of up to 2500 rpm.
First porous amorphous metal (2003)
~85 vol%, 200‐1000 μm
Review of the state of the art in the processing of BMG foams II
· Wada and Inoue open‐cell structures
(2003) by casting Pd42.5Cu30 Ni7.5P20 into beds of NaCl particles, quenching, and removing the salt by dissolution.
(a and b) SEM images of the surface structure of the porous Pd35Pt15Cu30P20glassy alloy rods with
porosities of 5 and 45% deformed up to strains of 0.2 and 0.05, respectively.
(2004) foamed this alloy by the expansion of
hydrogen bubbles precipitated from a supersaturated melt.
~65 vol%, 125‐250 μm
Review of the state of the art in the processing of BMG foams III
· Brothers and Dunand (2004)
the first amorphous foam using a commercial alloy, Zr57Nb5Cu15.4Ni12.6Al10 (Vit106), which was produced
by melt infiltration of beds of hollow carbon microspheres.
Optical micrographs showing the structure of syntactic Vit106 foam:
a) Low magnification image demonstrating foam uniformity;
b) Magnified image of the surface showing microscopic foam structure.
Misshapen carbon microspheres are visible, as is a sphere wall
fragment (indicated by Arrow). Good wetting is inferred from the lack of inter‐particle porosity.
· (2005), Brothers et al
demonstrated the use of the replication method for
amorphous foams, in which liquid Vit106 was infiltrated into a packed bed of leachable BaF2 salt particles that was removed after solidification in an acid bath.
Two other powder‐based methods:
· (2006) Xie et al: reported amorphous Zr55Cu30Al10Ni5with up to 67% porosity produced by partial spark‐plasma consolidation of amorphous powders with diameters of 37–53 mm.
· Hasegawa et al
studied the effects of lower levels
(approximately 2%) of porosity retained in melt‐spun ribbons of the same alloy, prepared from powder compacts
containing aluminum nitride.
AlN + Zr BMG → ZrN+Zr BMG+N2bubble
SEM micrographs of the transverse (mechanically crushed) cross section of the sintered porous Zr55Cu30Al10Ni5bulk glassy alloys with porosities of 4.7% (a), 33.5% (b), and the original powder (c).
SEM image of the bending fracture surface of a glassy composite alloy ribbon. Synthesized ZrN is indicated by arrows.
Review of the state of the art in the processing of BMG foams IV
· (2006), Jayaraj et al
reported successful processing of nanoporous Ti‐based amorphous metal ribbons using a method proposed in 2004 by Gebert et al. for a La‐based metallic glass, in which one phase is selectively acid‐leached from a two‐phase amorphous metal.
SEM images showing the formation of porous morphology of Y20Ti36Al24Co20two‐phase amorphous alloy. (a)–(c) Chemically dealloyed Y20Ti36Al24Co20 alloy in 0.1 M HNO3 solution for 24 h:
(a) low magnification demonstrating pore formation;
(b) magnified image showing three‐
dimensionally connected open type pores;
(c) crosssection of the dealloyed ribbon specimen.
(d) Electrochemically dealloyed Y20Ti36Al24Co20 alloy in 0.1M HNO3solution with an applied voltage of 1.9 V for 30 min.
Review of the state of the art in the processing of BMG foams V
First nano prous amorphous metal
Fully interconnected porosity/ 15‐155 nm
· (2006) Lee and Sordelet
where the sacrificial phase is crystalline rather than amorphous, and the starting two phase material is formed by warm extrusion of powder blends rather than casting.
SEM images of porous Cu47Ti33Zr11Ni8Si1 MG. Pores are uniformly distributed throughout the sample.
(a) Transverse polished cross section of Cu47Ti33Zr11Ni8Si1 MG + Cu composite precursor before dissolution of the Cu;
(b) macrostructure of porous Cu47Ti33Zr11Ni8Si1MG;
(c) transverse cross‐sectional microstructure
of porous Cu47Ti33Zr11Ni8Si1 MG;
(d) enlarged image of (c);
(e) longitudinal microstructure of porous Cu47Ti33Zr11Ni8Si1MG;
(f) detailed microstructure obtained from the lateral surface of the porous Cu47Ti33Zr11Ni8Si1MG.
Review of the state of the art in the processing of BMG foams VI
Images of several representative porous amorphous metals, produced using liquid‐state methods, are shown in Figure 1.
These methods demonstrated the possibility of foaming reactive Zr‐based alloys of the sort used in most metallic glass applications.
Representative powder‐processed porous amorphous metals are shown in Figure 2.
Mechanical Properties (1)
The primary purpose of introducing porosity in amorphous metals is to hinder the propagation of shear bands.
Two main mechanisms of hindering shear‐band propagation have been identified : shear‐band disruption and shear‐band stabilization.
The effectiveness of porosity in improving ductility and energy absorption in amor. metals, several compressive stress–strain curves for porous amorphous metals with porosities between 3.7% and 82% are shown in Figure
With increased porosity, the amorphous samples show decreasing strength and stiffness
i) shear‐band disruption
(the same mechanisms active in amorphous metal‐
matrix composites) : Pores (like solid inclusions) interrupt shear bands when their paths intersect, favoring branching of those bands and/or nucleation of new bands.
ii) shear‐band stabilization
(first noted during bending of thin amor. metal wires and foils) a) each band relaxes the stress from a smaller volume of the surrounding glass, enabling a closer spacing of the neighboring shear bands subsequently initiated, thereby increasing band density and overall plastic strain.
b) shallower shear bands produce smaller shear offsets at the surfaces of the wires or foils, and these smaller offsets reduce the probability of nucleating a crack. In the case of Zr‐based alloys, shear‐band stabilization becomes
noticeable for wire or foil thicknesses below about 1 mm.
Available data for the compressive yield strength and loading stiffness of porous amorphous metals are compiled in Figure porous amorphous metals span a wide range of strengths, from less than 10 MPa for high‐porosity foams to nearly 2 GPa for near‐dense alloys.
A more comprehensive illustration of
compressive ductility in porous amorphous metals is shown in Figure where failure
strains are compiled as a function of porosity.
pore morphology & the effectiveness that determine the effectiveness of the
ductilizing mechanisms_ some structures lead to almost no ductilization even at relatively high porosity.
• Porosity can be used as a means of selectively and continuously trading strength and stiffness for ductility, weight reduction, and energy absorption
(monolithic alloys crystalline metal)
• Porous amorphous metals could find use in a variety of applications, from structural materials to energy absorption or packaging applications
· The intrinsic benefits of AM
Large elastic energy return, wear resistance, and corrosion resistance and so on.
Low tensile ductility, cooling rate, high costs
Resistance to fatigue and tensile fracture High strength & compressive application
only small relative losses in strength At larger porosities, better energy absorption capacity, when compared on a volumetric basis, than crystalline Al‐based foams
Porous amorphous metals represent a promising new step toward the engineering application of amorphous metals by enabling mechanical properties and density to be varied
across a wider range than is possible using monolithic alloys or composites.
• compressive failure strains
can be varied from near‐maximum values
• compressive strength and stiffness
can be varied from ~2% to more than 80%
Porosity introduction can optimize
density‐compensated mechanical properties and tailor other properties
such as fluid permeability, specific surface area, and acoustic damping.